Two-dimensional semiconductors have attracted much interest in the last decade as a new material platform for valleytronics and optoelectronics , , , . Particular attention has been devoted to monolayer (ML) transition-metal dichalcogenides (TMDs), which are formed by a layer of transition-metal atoms [such as molybdenum (Mo) and tungsten (W)] sandwiched between two layers of chalcogenide atoms [such as sulfur (S) and selenium (Se)], with the metal and chalcogen atoms occupying the A and B sites of a hexagonal lattice (Figure 1). Exciton resonances in Mo- and W-family materials exhibit distinct optical properties because of their different spin orientations in the lowest conduction bands. In Mo-based TMD monolayers, the lowest exciton resonance is a dipole-allowed transition, while this transition corresponds to dark excitons in W-based TMD monolayers , . These materials feature a combination of unique optical properties. Their electronic bandgap lies in the visible and infrared, and as the layer thickness is reduced, the electronic band structure changes significantly , . In some TMD materials (e.g. MoS2), an indirect-to-direct gap transition occurs when a bilayer is thinned down to a monolayer , , , thus strongly enhancing light emission and absorption in the MLs.
Mobile excitons in TMD monolayers exhibit large binding energy and oscillator strength, leading to strong resonant coupling to light , , , , , . In addition to mobile excitons, ML TMDs can also host localized excitons that are bound to the defects and behave as spectrally narrow single-photon emitters , , . These localized emission centers often appear at the ML edges, but they can also be created or enhanced at specific positions by locally engineering the strain. Moreover, excitons form at the K and Kʹ points located at the Brillouin zone boundary. Because of the broken inversion symmetry of the ML and the strong spin–orbit coupling, the electronic states of the two K and Kʹ valleys have opposite spins, leading to spin-valley locking , , . Because of the valley-contrasting optical selection rule, the valley index can be addressed and manipulated by light. Optoelectronic applications of TMDs are often limited by their low quantum yield. Improving the quantum yield of TMD monolayers remains therefore an active and important area of research , . Additionally, light emitted from mobile or localized excitons needs to be efficiently collected and properly routed on chip for any integrated application.
In this review, we discuss how plasmonic nanostructures are particularly well suited for enhancing the optical properties of TMD MLs. Because of their two-dimensional nature, TMD MLs can be positioned very close, and optimally aligned, to a metallic structure. We have chosen to focus on emerging new directions in controlling a single emitter and valley index using plasmonic structures, and we anticipate rapid developments in these areas in the next few years. Because of the vast body of literature on TMD monolayers and many excellent reviews, we have omitted several interesting topics, including light–matter interaction in the strong coupling regime leading to the formation of polaritons , . In Section 2, we briefly summarize the optical properties of TMD monolayers and the use of plasmonic nanostructures to control spontaneous emissions. In Section 3, we discuss different approaches to increase emission from mobile or localized excitons into either free space (mediated by plasmonic antennas) or plasmonic waveguides for on-chip propagation. In Section 4, we focus on recent experiments where the chirality of plasmonic fields is combined with the valley-selective response of TMD materials to increase valley polarization, direct valley-selective emissions, and a spatially separate valley index by exploiting exciton–plasmon coupling.
2 Basic concepts
2.1 Excitons in TMD monolayers
Excitons in TMD monolayers have several unique properties, including a small Bohr radius as well as large binding energy and oscillator strength , , , , . Assuming a simple hydrogenic model, the nth exciton resonance binding energy in 2D materials is determined by
where μ is the reduced mass
Deviation from this simple model has been explicitly observed in WS2 monolayers . Nevertheless, it provides a simple estimate of the exceptionally large exciton binding energy in TMD monolayers, which has been determined to be a few hundred milli-electron volts , , , , or nearly two orders of magnitude larger than in conventional semiconductor quantum wells , . This large binding energy originates from an increased effective mass  and the insufficient screening in the direction perpendicular to the 2D plane (Figure 2) and, consequently, an enhanced Coulomb attraction between electrons and holes and a small Bohr radius , , , , , , . The large binding energy of excitons, trions (an exciton bound with an extra electron or hole ), and higher order bound states such as biexcitons ,  make these many-body states relevant for various optoelectronic devices, even at room temperature , , , .
A small exciton Bohr radius leads to a large spatial overlap between the electron and hole wavefunctions and, therefore, a large oscillator strength as manifested in the strong exciton absorption (i.e. 5–10% for TMD monolayers). A large oscillator strength should, in principle, lead to a rapid radiative decay. Calculations suggest that the exciton radiative decay is on the order of a few hundred femtoseconds in perfect TMD monolayers , . Deviations from ideal crystals lead to exciton localization and likely a longer exciton radiative lifetime. Directly measuring this radiative lifetime is difficult because commonly available techniques, such as pump/probe and time-resolved photoluminescence (PL), can only measure the total lifetime, determined by both radiative and nonradiative processes (we will discuss further this problem in Section 2.4). In addition, these experiments cannot distinguish intrinsic exciton recombination processes from those that repopulate the exciton resonances. Measurements often report a temperature- and excitation intensity-dependent exciton decay time, related to exciton–phonon and exciton–exciton interactions , , , , . Ultrafast spectroscopy measurements have suggested that the total exciton recombination lifetime at low temperature is ~1 ps or shorter , . This total lifetime is limited by the nonradiative decay because of the low quantum yield of commonly available TMD monolayers. Earlier measurements reporting longer lifetimes , ,  were often limited by the temporal resolution of the technique. Exciton thermalization process following an impulse excitation further complicates the interpretation of the measured exciton decay times . Placing TMD monolayers near plasmonic nanostructures likely shortens the lifetime further, making it even more difficult to accurately measure it. Explicit measurements of these dynamics in hybrid TMD–plasmonic materials are largely missing in the existing literature, despite being critical for enhanced light emission and modified valleytronic phenomena. The large oscillator strength also facilitates strong coupling to light, as reported in various coupled TMD–plasmonic systems , .
2.2 Single-photon emitters in TMD monolayers
Localized excitons, with completely different properties than 2D excitons, are also found in TMD monolayers. Indeed, several groups have reported that defects hosted in TMD monolayers (especially WSe2) can trap excitons, and their subsequent radiative recombination features good single-photon emission properties at low temperature , , , , . These excitons are typically localized at the flake edges and give rise to sharp emission lines (line widths ~100 μeV) that are red-shifted by 40–100 meV from the delocalized valley excitons  (Figure 3A). The quantum statistical properties of these single-photon emitters have been characterized by second-order photon correlation measurements , , , , and the measured lifetimes range from hundreds of picoseconds to few nanoseconds, similar to the values typically found in InAs self-assembled semiconductor quantum dots . This long lifetime is in strong contrast with the short lifetime (~1 ps) of unbound excitons in ML TMDs, which is typically dominated by nonradiative decays.
High-resolution magneto-optical measurements have shown that the emission from these localized excitons is composed of a doublet (Figure 3B), which features orthogonal linear polarizations , , , . When a magnetic field is applied perpendicular to the monolayer plane, the doublet splitting increases (Figure 3C) and the emission polarization evolves from linear to circular ; the handedness of circular polarization can be controlled by the magnetic field sign . No clear dependence of the splitting and polarization on the magnetic field is observed when the field is parallel to the plane, similar to the case of unbound excitons.
The nature of these defects is not fully understood yet. It has been suggested that they can be due to vacancies, impurity atoms, or local strain . Indeed, the defects initially investigated appeared mainly close to the edge of the monolayer, which limits their potential in practical applications. Many groups have therefore investigated the possibility of deliberately creating these defects with controlled positions. It has been shown that by placing ML TMDs on dielectric  or metallic ,  nanopatterned substrates, it is possible to induce a local strain pattern in the monolayer, which results in an array of quantum emitters. Palacios-Berraquero et al. , for example, deposited a WSe2 monolayer on an array of silicon micropillars (Figure 3D). The PL intensity was highly enhanced at the position of the pillars (Figure 3E), and the PL spectra showed sharp single-photon emission lines (Figure 3F) with characteristics similar to those of emission centers randomly located at the flake edges.
2.3 Valley index in TMD monolayers
Valley refers to the energy minima or maxima in the electronic band structures, typically corresponding to the high-symmetry points in the reciprocal space of crystal , , , , , . While these valleys play an important role in electronic transport processes and optical transitions, the valley signature does not directly couple to external stimulants (e.g. electric or magnetic fields) in a specific way. Thus, it is usually not possible to manipulate the degree of freedom of the valley. In monolayer TMDs, the valley-contrasting optical selection rules allow creating electrons, holes, or excitons with a particular valley index using circularly polarized light . Indeed, excitons are formed at the corner of the Brillouin zone at two inequivalent valleys (Figure 4A), which are related to each other via time-reversal symmetry , , . This binary degree of freedom has been proposed as an alternative way to represent information , , , similar to charges and spins. Upon optical excitation with circular polarization (e.g. σ+), excitons or trions are created in one particular valley (e.g. the K valley). The degree of valley polarization can be quantitatively evaluated by
Earlier experiments had reported that the subsequent PL maintains the chirality of the excitation source if the proper excitation laser wavelength is chosen , , , , inferring that the exciton valley index can act as a robust degree of freedom to carry information (Figure 4B). However, it is important to distinguish valley polarization associated with free carriers and the one with optical transitions such as excitons or trions , , , , , , . The valley polarization of free carriers is long-lived because of the large energy splitting between states with opposite spins due to strong spin–orbit coupling in TMDs. Optical manipulation of valley index often relies on resonant excitations of excitons or trions. The valley polarization and coherence associated with excitons are quickly lost (~1 ps) as a result of the strong electron–hole exchange interaction , , . In order to observe circularly polarized PL, the exciton valley polarization needs to be comparable to the exciton recombination lifetime, which is found to be typically ~1 ps (at low temperature) or shorter in TMD monolayers , . This short lifetime is consistent with the large oscillator strengths or dipole moments associated with exciton transitions. Valley polarization associated with trions can be long under proper excitation conditions .
2.4 Control of the spontaneous emission with plasmonic structures
A quantum emitter generally radiates into all available photonic modes, and its radiative decay (i.e. decay accompanied by photon emission) competes with nonradiative channels. For an emitter placed in a bulk environment (indicated by the superscript 0), its total decay rate is given by the sum of the radiative (r) and nonradiative (nr) decay rates,
The bulk radiative decay rate
Such control of the radiative process is possible because the radiative decay rate is not an intrinsic property of the emitter but depends on the local density of optical states (LDOS) available at the position and emission frequency of the emitter . The LDOS, in turn, depends on the vacuum electric field created by the considered nanostructure. As a result, when an emitter is placed in a nonhomogeneous environment (such as an antenna or a cavity), its radiative decay rate is modified from
Thus, only when the nonradiative and metal-induced decay rates are negligible can the Purcell factor be easily connected to the total decay rate enhancement. Moreover, when γM≈0, a measurement of the total decay rate enhancement gives always an underestimate of FP(r). A precise measurement of FP(r), therefore, requires the knowledge of the emitter’s quantum efficiencies in the bulk and in the inhomogeneous environment.
In the simplest scenario where only one optical mode dominates the LDOS, the maximum achievable radiative enhancement is given by the well-known Purcell formula
Plasmonic modes are created by coherent oscillations of electrons in noble metals or heavily doped semiconductors, which couple strongly to the electromagnetic field and form polaritons. For extended surfaces, this results in waves termed surface plasmon polaritons (SPPs), which are tightly confined to the metal–dielectric interface and propagate along it. For metallic nanoparticles, the confined oscillation of the electrons gives rise to the localized surface plasmon resonances (LSPRs). The spectral response of LSPRs can be largely tailored by changing the particle shape and dimensions. Because of their capability of coupling a near-field source with far-field radiation (and vice versa), metallic nanoparticles are often termed plasmonic antennas in analogy with their radio wave counterpart , , , . The electric field of plasmonic modes is strongly confined near the nanoparticle surface, leading to large field enhancements and ultra-small mode volumes, which are not diffraction-limited: volumes smaller than 10−3λ3 have been demonstrated in nanodisk resonators . Therefore, despite their low Q factor due to the unavoidable Ohmic losses, plasmonic modes can still largely boost the ratio Q/V and lead to high Purcell enhancements while at the same time maintaining large radiative decay rates; in a recent experiment with silver nanocubes , total decay rate enhancements larger than 1000 were obtained, together with comparable or even higher enhancements of the radiative decay rate. Moreover, a low Q increases the operational bandwidth, which leads to two key advantages. First, it facilitates the spectral alignment between the emitter and the plasmonic mode, removing the need for post-fabrication tuning (which is often necessary for high-Q dielectric resonators). Second, due to the spectrally broad plasmonic resonance, a simultaneous enhancement of the nonresonant excitation field in PL experiments is also possible, further boosting the collected PL intensity.
While beneficial for the radiative decay rate enhancement, the ultra-small mode volumes of plasmonic resonators introduce a practical challenge for enhanced light–matter interactions. Since the electric field decays exponentially away from the particle surface (with a typical decay length of few tens of nanometers at optical frequencies), an emitter needs to be very close to the metal and optimally aligned to couple efficiently. This requirement has so far strongly limited the coupling of plasmonic structures with solid-state semiconductor emitters, such as quantum dots (QDs). Indeed, these emitters are usually embedded in a hosting 3D matrix, which therefore sets a minimum distance between the emitter and the metallic surface. Semiconductor quantum dots (SCQDs) in III–V materials, for example, need to be buried at least 30 nm below the surface to avoid a large increase of the nonradiative recombination rates . This problem can be partially solved by passivating the surface , but the unavoidable embedding matrix still leads to limited , ,  or absent  Purcell enhancements.
These challenges are absent when monolayers of TMDs are used as an active material: here, excitons are naturally embedded in a 2D sheet, and they can therefore be placed within few nanometers from a metallic surface. Recent experimental works have demonstrated PL enhancement larger than 10× with different geometries , ,  and increase of the radiative decay rate larger than 300× in optimized resonators , , . Moreover, the reduced dimensionality of the hosting matrix offers greater flexibility in terms of positioning and orienting the emitters with respect to the optical field, which can be exploited to reach an optimal alignment between the dipole moment and the plasmonic field .
3 Coupling emitters in TMD monolayers to plasmonic nanostructures and metasurfaces
In this section, we discuss different implementations that have been proposed and demonstrated in recent years to couple TMD monolayers to plasmonic antennas and devices. We will focus in particular on works where plasmonic-induced enhancement of photoluminescence and decay rate have been shown. In Table 1, we summarize the results of the studies reviewed in this section.
Summary of the performance of several plasmonic/TMD systems discussed in the text.
|Plasmonic structure/TMD material||Temperature||Spectral feature investigated||Peak PL enhancement||Modified lifetime||Decay rate/Purcell enhancement||Reference|
|Plasmonic structures fabricated on top of TMD monolayers|
|Ag bowties/MoS2||RT||ME||16× (A), 25× (B). EE=1.8×||–||–|||
|Au bowties and dimers/MoS2||RT||ME||8× (bowties) 6× (dimers)||–||–|||
|Ag slot antenna/WSe2||RT||ME||700×, EE=2.2×a||–||~300a|||
|TMD monolayers draped over plasmonic structures|
|Ag nanotriangles and islands/WSe2||LT (10 K)||ME (~705 nm) and LE (>720 nm)||20× (LE/nanotriangles)|
Quenching of ME
|Si–Au–Al2O3 nanopillars/WSe2||LT (3 K)||Induced LE (>720 nm)||2×||2.2 nsb||2.4b|||
|Ag MIM waveguide WSe2||LT (3 K)||Induced LE (>720 nm)||–||3.34 nsc||1.8c|||
|Au nanocubes/WSe2/Au mirror||LT (4 K)||Induced LE (750–800 nm)||–||266±120 psd||181d|||
We only included works where enhancements of photoluminescence (PL) or decay rate were reported. In the column “Decay rate/Purcell enhancement”, the accompanying footnote specifies for each case which of the two enhancements is reported and how it is calculated. When available, we have indicated the fraction of the PL enhancement due to the enhancement of the excitation (EE).
aThe excitation enhancement (EE) includes also the enhanced collection efficiency. The decay rate enhancement was not obtained through time-resolved measurements, but estimated from the PL enhancement and the numerically calculated antenna efficiency and quantum yield.
b“Modified lifetime” is the average over 48 different emitters interacting with plasmonic nanopillars. The decay rate enhancement is calculated by dividing the modified lifetime by the average lifetime of 39 emitters in a bare flake.
c“Modified lifetime” is the average over seven different emitters located on the waveguide. The decay rate enhancement is calculated by dividing the modified lifetime by the average of the lifetime of 10 emitters in a bare flake.
3.1 Coupling of mobile excitons to plasmonic antennas
A well-investigated approach to couple ML TMDs to plasmonic antennas consists in fabricating the metallic structures directly on top of the TMD layer with conventional lithographic techniques. Several groups have used this method to study plasmonic-induced PL enhancement of mobile excitons in TMD monolayers , , . Butun et al.  placed square arrays of silver nanodisks on top of a MoS2 monolayer (Figure 5A) and measured the room-temperature PL from the A exciton in MoS2 in the spectral range 650–750 nm. PL enhancements larger than 10× were found for some nanodisk diameters (Figure 5C). Moreover, the maximum enhancement occurs at a particular emission wavelength, which red-shifts as the nanodisk diameter increases (Figure 5B); thus, while a contribution from excitation enhancement cannot be ruled out, the observed PL enhancement is necessarily related to an increased efficiency of the emission into the plasmonic resonance of the single nanodisk. Similar values of PL enhancements were also reported by Lee et al.  in samples made of a square array of silver bowtie antennas placed on a MoS2 monolayer (Figure 5D, E). Palacios et al.  fabricated 40-nm-thick gold dipole and bowtie antennas on top of a MoS2 monolayer. The maximum PL enhancement depended sensitively on the in-plane dimensions and was found to vary from 1.4 to 4.5 for the dipole antennas and from 4.1 to 8.40 for the bowtie antennas. No marked correlation between the antenna dimensions and the wavelength at which the maximum PL enhancement occurs was found, indicating that, in this experiment, the plasmonic structures mainly provided a nonresonant excitation enhancement.
A different approach, which ensures self-alignment between a nanostrip monolayer of WSe2 and a slot antenna, was recently proposed by Eggleston et al.  (Figure 5F–I): the TMD monolayer was deposited on a sacrificial substrate and covered by SiOx; a lithographically defined mask was then used to etch away the TMD/SiOx everywhere except on small rectangular strips. Without removing the mask, a thick layer of silver was evaporated on the sample, thus realizing a metallic slot cavity automatically aligned with the TMD strip (Figure 5F). Because of the high electric field enhancement at the TMD position (Figure 5G), and because of the fact that any portion of the TMD layer outside the antenna was removed, a very large PL enhancement was obtained, up to ~700× (Figure 5H, I). The PL enhancement was maximized when the plasmonic resonance supported by the nanoslot was tuned to the peak wavelength of the exciton emission (Figure 5H, I, A1 curve). The total enhancement was due to a combination of increased excitation, improved collection efficiency, and higher radiative decay rate. The authors estimated numerically that the antenna was able to redirect 48% of the radiation into the objective numerical aperture, compared to a value of 17% for a bare sample. This effect, combined with a small pump enhancement (and the fact that only the dipole moments in the material parallel to the slit contribute to the enhancement), led to an overall enhancement of the collection efficiency by 2.2×. The radiative emission enhancement was therefore estimated to be 318×.
3.2 Coupling of defect-bound excitons to plasmonic structures
A different approach to realize coupled TMD–plasmonic systems consists in draping a TMD monolayer over a nanopatterned substrate. Several works have used this method with dielectric  or metallic structures , , , , and it has been suggested that the strain induced in the TMD layer by the substrate creates local potential minima, leading to localization centers for excitons.
Johnson and coauthors  investigated a sample composed of WSe2 flakes transferred on to either a silver nanotriangle array, a uniform silver island, or a bare SiO2 substrate (Figure 6A, B) and measured the low-temperature PL in the three different cases. The single triangles support a broadband, localized plasmonic resonance centered at 645 nm, which partially overlaps with the emission from the mobile (~715 nm) and the localized (>720 nm) excitons in WSe2. The authors found that the emission from the localized excitons was enhanced by the metal environment: the low-temperature (10 K) PL enhancement (spectrally integrated in the range 720–80 nm and calculated with respect to the case of a bare SiO2 substrate) was found to be ~8× for the Ag island and ~20× for the nanotriangle array. When considering the actual area occupied by the nanotriangles, the normalized enhancement factors increased to ~200×. This large enhancement was likely due to a combination of decay rate enhancement and increased light absorption, but the lack of lifetime measurements prevented the quantitative evaluation of the two contributions separately. Remarkably, the authors observed that the emission from the mobile excitons was, instead, quenched when the WSe2 ML was on the plasmonic structures (either on the Ag film or Ag nanotriangle array). This observation is consistent with the different relaxation dynamics for the mobile and localized excitons. The PL spatial maps acquired in this work showed that the defect-bound emitters were mainly localized at the flake edges and that the strain induced by draping the WSe2 layer on the nanotriangles did not create additional defects.
A similar approach has been used by different groups to demonstrate that the strain induced by a nanopatterned array could be used to obtain ordered arrays of quantum emitters. Iff et al.  utilized square arrays of gold nanopillars on a SiO2 layer with conventional lithography techniques. The array pitch was large enough (4 μm) so that each pillar could be addressed individually in optical experiments. An atomically thin layer of WSe2 was then transferred onto the pillar array (Figure 6D). For most of the nanopillars, this resulted in a locally strained layer, leading to a tent-like structure (Figure 6E). A spatially resolved PL study showed a high correlation between bright emission spots and the position of the metallic pillars (Figure 6G). The low-temperature emission spectrum featured several sharp peaks below the free exciton energy (<1.74 eV) (Figure 6F), which the authors associated with strongly localized excitons due to strain. Second-order autocorrelation measurements (Figure 6H) showed g(2)(0)=0.17 and confirmed the single-photon emission from these peaks. Moreover, for asymmetric pillars, a strong correlation between the polarization of light and the long axis of the pillar was found (see Figures 6I and 3D in Ref. ), indicating that the exciton emission was strongly modified by the localized plasmonic mode. Cai and coauthors utilized a similar system composed of hybrid dielectric–metallic nanopillars (Figure 6J, K) to demonstrate enhancement of the decay rate of the localized excitons . The low-temperature PL spectra from each nanopillar showed one or multiple narrow peaks, indicating the formation of localized emission centers, whose single-photon nature was confirmed by g(2)(0) measurements. The nanopillar design was optimized to induce a large Purcell factor (>50) for an emitter positioned on top of it and emitting at 780 nm (Figure 6L). The authors measured the lifetime of 46 single-defect emitters located on the plasmonic nanopillars (Figure 6M, top). They then compared these to a similar number of emitters in two control groups, one with dielectric nanopillars without gold (Figure 6M, middle) and the other in the bare material with no nanopillars (Figure 6M, bottom). The average lifetime of the emitters in the bare material (T=5.3±2.3 ns) was not statistically changed for the emitters interacting with non-plasmonic nanopillars (T=5.2±2.1 ns). The average lifetime of the emitters interacting with the plasmonic nanopillars was, instead, reduced to T=2.2±1.5 ns, indicating an enhancement of the total decay rate of 2.4.
In most studies discussed so far (and in the next section), the PL and decay rate enhancements have been calculated by averaging the lifetimes of ensembles of emitters coupled and uncoupled with a plasmonic structure, and modest values of decay rate enhancements have been demonstrated. In a recent experiment, Luo and coauthors have demonstrated a method (inspired by Ref. ) to achieve large radiative enhancements and, at the same time, to measure the bare and enhanced decay rates of the same emitter . A WSe2 was transferred onto an array of gold nanocubes fabricated on a sapphire substrate, and a gold flat layer was then attached on the other side (Figure 6N). The vertical plasmonic gap mode obtained featured a very large field enhancement near the nanocube edges (Figure 6O). The low-temperature PL spectra acquired from each nanocube showed a set of sharp peaks in the 755–790 nm spectral region (Figure 6P). In most cases, exactly four spectrally isolated emitters were found per site, leading the authors to suggest that each corner of a nanocube was coupled to one quantum emitter. The lifetime of each emitter was measured before and after placing the flat gold layer, thus allowing the lifetime variation of each emitter to be evaluated. The authors found that the lifetime could be reduced by a factor as high as 57 (Figure 6Q), which led to a Purcell factor of 551 after correcting for the variation of the quantum efficiency.
3.3 On-chip guiding of single photons extracted from TMD materials
As discussed in the previous section, several works have demonstrated the coupling of light emitted by either localized or mobile excitons in ML TMDs to plasmonic nanocavities or arrays. However, the light collected by these structures is then re-emitted directly into the far field, thus hindering any application for plasmonic circuitry and, in general, for on-chip manipulation of the optical signal. The possibility of coupling defect-bound excitons to propagating surface plasmons has been demonstrated in a few recent works. In the work of Cai et al. , a sheet of atomically thin WSe2 was transferred onto the top of a chemically synthesized silver nanowire (Figure 7A). The strain induced by the nanowire created localized and optically active defects in the WSe2 layer, as demonstrated by a spatial map of the PL intensity (Figure 7B). The low-temperature emission spectrum (Figure 7C) featured several sharp lines, each consisting of a doublet corresponding to the two different in-plane polarizations of the localized exciton. The single-photon nature of the emission was proven by a second-order correlation measurement of the emission into free space (Figure 7D). Because of their proximity, these defects coupled efficiently to propagating surface plasmons sustained by the nanowire. Upon laser excitation at the nanowire center (point C in Figure 7E), emission was also observed from the nanowire ends (points A and B). Importantly, while the emission from the nanowire center showed the doublet structure mentioned above (Figure 7F, top panel), the emission from the nanowire ends showed only one peak (Figure 7F, center and bottom panels). The authors attributed this behavior to the fact that, due to their different polarizations, only one of the two quasi-degenerate localized excitons coupled efficiently to the nanowire and propagated from the center to the edges. By measuring the intensity of light emitted from the nanowire ends for 21 different nanowires, the authors estimated an average coupling efficiency of 26%±11%. In this approach, the coupling efficiency was affected by an unfavorable plasmon–exciton geometrical alignment (Figure 7M): the electric field vector of the nanowire plasmonic mode is mainly perpendicular to the metal surface and directed radially outward, while the excitons have in-plane dipole moments, tangential to the metal surface. Because of this poor alignment, no enhancement of the decay rate was observed in this study. In order to improve the coupling, the same group demonstrated a different design based on a metal–insulator–metal waveguide (Figure 7G–L) . Two silver rectangular stripes, separated by a small air gap, were fabricated on top of a SiO2 substrate, realizing a slot waveguide. The electric field of the resulting guided mode is strongly localized in the air gap and, importantly, its main component is in plane and orthogonal to the waveguide direction. Thus, when a WSe2 monolayer was transferred onto the top of the structure, the dipole moment of a defect-bound exciton in the air gap region was quasi-optimally aligned to the electric field of the guided mode (Figure 7N). Similar to the case of the nanowire, the emission spectrum from the excitons was a doublet (Figure 7I), and only one of the two emission peaks was visible when collecting light from the opposite end of the waveguide (Figure 7J) as a result of the different in-plane polarizations. By measuring the lifetime of 10 emitters located on the pristine monolayer and 7 emitters located on the waveguide/monolayer (see Figure 7K, L for representative measurements), the authors estimated a lifetime reduction of ~2.
4 Coupling valley index to plasmonic nanostructures and metasurfaces
4.1 Enhancing valley polarization with plasmonic nanostructures
Because of the low quantum efficiency of available TMD monolayers , , the PL intensity can be drastically enhanced by placing a monolayer near plasmonic antennas in various geometries, such as bowtie or gap plasmons, as was shown in the experiments reviewed in the previous sections. Enhancing exciton valley polarization, on the other hand, requires a more careful design of the near field. There are a number of reasons why the presence of a plasmonic nanostructure or a metasurface can enhance valley polarization. In addition to shaping the polarization of the near field, the presence of a plasmonic structure may shorten the exciton recombination lifetime via the Purcell effect while having minimal influence on valley scattering time.
In a recent work, Ziwei and coworkers  investigated a sample composed of a MoS2 monolayer sandwiched between a chiral metasurface and a Au film (Figure 8A). The scanning electron microscopy (SEM) images of the metasurface and of the hybrid structure are shown in Figure 8B and C, respectively. In the absence of a metasurface, a finite valley polarization ρ~25% was observed in PL for both σ− and σ+ excitation conditions with the excitation wavelength of 633 nm and at 87 K (Figure 8D, G and blue circles in Figure 8F, I). For the hybrid TMD–plasmonic structure, at the A exciton energy around 665 nm, ρ increased to 43% with σ− excitation (Figure 8E and blue circles in Figure 8F), while it decreased to 20% with σ+ excitation (Figure 8H and blue circles in Figure 8I). This result can be explained by considering the exciton dynamics in the hybrid structure. For K′ valley excitons, both the generation and emission rates of excitons are enhanced as a result of the interaction between the MoS2 monolayer and the metasurface. In contrast, K valley exciton emission is suppressed. Meanwhile, the intervalley scattering rate mainly depends on the temperature and the excitation wavelength, thus largely unchanged in the presence of the metasurface. The enhanced or reduced exciton valley polarization results from the competition of exciton generation, emission, and the intervalley scattering rate.
4.2 Directing valley exciton emissions
Plasmonic antennas have been shown to significantly modify the emission rate, radiation pattern, and sometimes the polarization, as discussed above. Plasmonic devices can also be used to direct emission from valley polarization excitons toward different directions, effectively serving as a link between photonic and valleytronic devices . A conceptually simple design has been proposed by Chen and coworkers  (Figure 9A). By coupling circularly polarized dipoles (i.e. valley excitons) to plasmonic antennas that support both dipole and quadrupole modes, the interference between the two plasmonic modes can be exploited to direct emissions from opposite valleys to different directions (Figure 9B). When the phase between dipole and quadrupole modes changes by π, the emission is directed to the opposite direction.
A metasurface designed to direct valley-selective emission from a monolayer WS2 has been demonstrated by Chervy and coworkers  (Figure 10A). The metasurface consists of a series of rectangular nanoapertures in a gold film rotated stepwise along one axis by an angle ϕ=π/6. These rotating apertures are further arranged in a square lattice with a grating period Λ, setting up a rotation vector of
The strong coupling between excitons and SPPs, due to the exceptionally large exciton oscillator strength, leads to the formation of polariton states, as evidenced by the anti-crossing dispersion in the angle-resolved absorption spectra , . The valley index is inherited by the exciton-SPPs. The PL from these chirality-dependent polariton states is separated in k-space resolved measurements, as shown in Figure 10B. Interestingly, the authors did not observe valley polarization from PL from a bare WS2 in the excitation conditions adopted. The enhanced valley polarization and valley coherence associated with the exciton-SPPs suggest that these hybrid modes may be more suitable for optical manipulation of valley index than excitons hosted in bare TMD monolayers.
4.3 Spatial separation of valley index
Another prerequisite to build valleytronic devices is the capability of separating carriers and quasiparticles with different valley indexes. Several strategies based on various Hall effects have been explored , , , , , . For example, the valley Hall effect in monolayer TMDs has been proposed  and later experimentally demonstrated . In this phenomenon, the valley-specific Berry curvature acts as a momentum-dependent synthetic magnetic bias, leading to transverse separation of valley-polarized free carrier driven by the in-plane electric field in the perpendicular direction. Very recently, the exciton valley Hall effect was demonstrated , where the valley-polarized excitons were separated in the presence of a laser-induced temperature and exciton density gradient. However, these previous valley separation schemes were demonstrated only at low temperature, thus limiting their use in practical applications.
4.3.1 Chiral photonics
In a different context, optical spin–orbit interaction enables the separation of optical spins and directional propagation of electromagnetic waves with chiral polarizations , , , . Such chirality-dependent propagation can be understood within a near-field interference picture . Consider a circularly polarized dipole (Px+iPz) placed in the vicinity of a waveguide surface, as illustrated in Figure 11A. This dipole excites the guided modes in the waveguide, with the horizontal component of the dipole (Px) driving the longitudinal field and the vertical component (Pz) coupling to the transverse field of the guided electromagnetic mode. The magnetic field Hy(kx) induced by Px(Pz) is symmetric (antisymmetric) respective to kx. Therefore, the linear superposition of the two orthogonal dipoles Px and Pz leads to a nonsymmetric spatial frequency distribution. The guided modes with kx>0 (kx<0) interfere destructively (constructively). This near-field interference is the mechanism for the chirality-dependent, unidirectional excitation of guided modes. As an example, Figure 11B shows the calculated magnetic field distribution at a metal/dielectric interface induced by a circularly polarized dipole. While both counter-propagating SPP modes are supported on the metal/dielectric interface, only one of these modes is predominantly excited by the circular dipole, leading to chirality-dependent SPP propagation.
The optical spin Hall effect provides a powerful tool to guide chiral photon propagation on chip, which is essential to realize this form of optical information transmission. Chirality-dependent unidirectional photon propagation has been demonstrated in hybrid systems, which combine semiconductor quantum emitters and waveguides . The chirality of the emitted photons is governed by the optical selection rules in the semiconductor QD. The direction of the photon propagation is controlled by a properly designed waveguide. Coles and coworkers demonstrated control of the direction of chiral photon emission by coupling a QD to a nonchiral waveguide (Figure 11C) . When the QD is positioned at the center of the waveguide, the emission intensities are the same for both directions (Figure 11D) as expected from the symmetry consideration of the nonchiral waveguide. In contrast, when the QD is displaced from the center, the in-plane mirror symmetry of the hybrid system is broken. As a result, the emission direction depends on the chirality, with σ+ photons preferentially propagating in one direction and σ− photons in the other direction (Figure 11D). In another example , Sollner and coworkers demonstrated chirality-dependent directional emission of a QD by coupling it to a specially designed waveguide with broken mirror symmetry, known as a glide-plane waveguide, as shown in Figure 11E. When coupled to a glide-plane waveguide, an excited QD with σ+ polarization transition dipole preferentially emits photons in one direction (Figure 11F). When the chirality reverses, so does the emission direction.
Considering these examples of chirality-dependent photonic devices and the valley-contrasting optical selection rules in TMD monolayers, it is natural to extend these approaches to realize valleytronic devices. In such a hybrid system, TMD monolayers act as the active component while photonic structures function as the passive components. For example, the spatial separation of excitons with a specific valley index may be realized by routing valley excitons facilitated by the optical spin Hall effect. Chiral photons emitted by valley-polarized excitons may be channeled toward different directions. Below, we review two recent works exploring such opportunities.
4.3.2 Plasmonic nanowires
Nanowires can harvest exciton emission with exceptionally high efficiency as previous studies on coupling QDs and plasmonic wires have demonstrated , . Taking advantage of this effect, a valley–photon interface has been realized by coupling a single silver nanowire to a few-layer-thick WS2 flake (Figure 12A) . The nanowire supports guided-SPPs possessing transverse optical spin angular momentum, which is locked with the propagation direction. The chirality-dependent directionality is illustrated in Figure 12B. A source positioned in the upper part of the nanowire (y>0) and emitting light with σ+ (σ−) polarization, will excite a SPP propagating to the left (right). The effect is inverted when the source is positioned in the lower part (y<0). Therefore, the chirality of the optical spin angular momentum is determined by a combination of the propagation direction and the y position.
Experimentally, valley-polarized excitons were locally excited in the middle of the silver nanowire (x=0) for different y positions with a circularly polarized laser of 594 nm. The K and Kʹ valley excitons are associated with in-plane circularly polarized dipoles oscillating with opposite helicity (Ex±iEy) . The transition dipoles from different valleys couple to the guided SPP modes propagating in opposite directions. The scattered PL at the end of the nanowire was detected on a charge-coupled device (CCD) after passing through a band-pass filter (620–630 nm), chosen to overlap with the exciton resonance in WS2.
The valley-dependent directionality is quantified by kexp≡[IL(y)–IR(y)]/[IL(y)+IR(y)], where IL,R(y) represent the PL intensity scattered at the left and right end of the nanowire as a function of y, as shown in Figure 12C, D. When the σ− excitation spot is above (below) the nanowire, i.e. at y<0 (y>0), the excitons couple to SPPs propagating to left (right) end of the nanowire. When the handedness of the excitation is reversed, so does the propagation direction. Note that the chirality-dependent propagation can only be achieved under asymmetric excitation condition in the transverse direction (i.e. y≠0) because of the symmetry of the nanowire. If the excitation laser spot is centered with respect to the nanowire (y=0), valley polarization separation vanishes. This sensitive dependence on the excitation position makes this scheme for spatial valley separation quite challenging for practical applications.
Metasurfaces with broken-mirror symmetry have been recently proposed to spatially separate valley excitons in TMDs at room temperature. The metasurface introduced in Ref.  consists of asymmetrical grooves arranged in a sub-wavelength period. Figure 13F shows the SEM image of the cross-section of the fabricated asymmetric grooves. In the case of symmetric grooves (Figure 13A), the mirror symmetry along the yz-plane leads to chirality-independent propagation, i.e. an in-plane dipole with left- or right-handed chirality couples to both sidewalls equally, similarly to the symmetric nanowire considered above. However, when the mirror symmetry is intentionally broken by tilting one side wall while keeping the other wall vertical, the guided SPPs (gSPPs) excited by valley exciton dipoles are different for vertical and tilted walls (Figure 13B), resulting in chirality-dependent, unidirectional propagation of gSPPs.
Experimentally, a linearly polarized laser at wavelength 532 nm was used to equally populate the two valleys in the monolayer MoS2 placed on top of the metasurface. The valley-excitons then induced chiral gSPPs propagating away from the laser excitation spot and re-excited excitons along its path. Such exciton-gSPP-exciton nonradiative energy transfer process separated the valley excitons spatially, as shown in Figure 13H, I. The g-SPP modes have an E-field with a significant in-plane component. Thus, the coupling between the in-plane dipoles associated with excitons in monolayer TMD and gSPPs can be rather efficient. The efficiency of the cascaded energy conversion process of the exciton-gSPP-exciton is calculated to be higher than 20%. In a control experiment, the researchers showed that such spatial valley separation was absent when the MoS2 monolayer was placed on a metasurface consisting of symmetric grooves (Figure 13J). The asymmetric metasurface can also direct valley exciton emission to different directions, serving as an interface between valleytronics and photonic devices similar to those discussed in earlier in this section.
The two examples chosen in this section have demonstrated that plasmonic antennas and metasurfaces can be used to control the valley index including the degree of valley polarization, the emission direction of valley polarized excitons, and the spatial separation of valley excitons. The performance of these hybrid photonic devices is determined by SPP propagation, ultrafast exciton dynamics, and how plasmonic nanostructures modify such dynamics via exciton–plasmon coupling. Because of the large oscillator strength of valley excitons in TMDs, a strong coupling between valley excitons and SPPs or LSRPs can be reached in properly designed plasmonic structures.
TMDs represent a new class of flexible photonic materials, hosting single-photon emitters with defined locations and extending optical control to a new quantum degree of freedom, the valley. Integrating these layered materials with plasmonic nanostructures, waveguides, and metasurfaces advances both classical and quantum photonics. There are a few clear future directions in this field of research. Proper waveguides that can guide single-photon emission efficiently and preserve the polarization states, which are often used to encode quantum information of flying qubits, have yet to be demonstrated. Addressing the long-standing challenge of loss in plasmonic materials will improve the performance of hybrid photonic devices. For example, the limited degree of valley polarization in the hybrid system can be improved by implementing new metasurface designs that can specifically couple to dark exciton states or reduce the energy concentration in noble metals.
With the rapid progress in synthesizing and fabricating van der Waals (vdW) heterostructures, new exciton resonances are identified. The interlayer excitons in vdW heterostructures exhibit long recombination and valley polarization times , , , , , . The long recombination lifetime suggests that their oscillator strength is small and couples relatively weakly to light. Such slow dynamics may also be related to indirect transitions in the momentum space. Plasmonic nanostructures placed near TMD heterostructures may lead to measurable changes in exciton dynamics by shaping the photon density of states and provide coupling to large photon momenta in the near field to brighten indirect transitions. Plasmonic nanostructures may provide a strong field enhancement, needed for optical switching of topological phases of matter , , . A metasurface may further define the optical properties of an array of identical single-photon emitters localized by an in-plane Moiré superlattice , .
LS was supported by NSF DMR-1306878, Funder Id: http://dx.doi.org/10.13039/100000078. JC was partially supported by the NSF MRSEC program DMR-1720595, Funder Id: http://dx.doi.org/10.13039/100000078, Grant Number: NSF DMR-1808042, which also facilitated the collaboration between XL and AA. XL acknowledges the support from the Welch Foundation via grant F-1662, Funder Id: http://dx.doi.org/10.13039/100000928. AA and MC acknowledge the Air Force Office of Scientific Research with MURI grant No. FA9550-17-1-0002, Funder Id:http://dx.doi.org/10.13039/100000181 and the Welch Foundation with grant No. F-1802, Funder Id:http://dx.doi.org/10.13039/100000928. MC was supported by a Rubicon postdoctoral fellowship by The Netherlands Organization for Scientific Research (NWO).
Novoselov KS, Mishchenko A, Carvalho A, Castro Neto AH. 2D materials and van der Waals heterostructures. Science 2016;353:aac9439.
Britnell L, Ribeiro RM, Eckmann A, et al. Strong light-matter interactions in heterostructures of atomically thin films. Science 2013;340:1311–4.
Malic E, Selig M, Feierabend M, et al. Dark excitons in transition metal dichalcogenides. Phys Rev Mater 2018;2:014002.
Baranowski M, Surrente A, Maude DK, et al. Dark excitons and the elusive valley polarization in transition metal dichalcogenides. 2D Mater 2017;4:025016.
Zhang C, Chen Y, Johnson A, et al. Probing critical point energies of transition metal dichalcogenides: surprising indirect gap of single layer WSe2. Nano Lett 2015;15:6494–500.
Mak KF, Lee C, Hone J, Shan J, Heinz TF. Atomically thin MoS2: a new direct-gap semiconductor. Phys Rev Lett 2010;105:136805.
Jin W, Yeh PC, Zaki N, et al. Direct measurement of the thickness-dependent electronic band structure of MoS2 using angle-resolved photoemission spectroscopy. Phys Rev Lett 2013;111:106801.
Ross JS, Wu S, Yu H, et al. Electrical control of neutral and charged excitons in a monolayer semiconductor. Nat Commun 2013;4:1474.
Berkelbach TC, Hybertsen MS, Reichman DR. Theory of neutral and charged excitons in monolayer transition metal dichalcogenides. Phys Rev B 2013;88:045318.
Lui C, Frenzel AJ, Pilon DV, et al. Trion-induced negative photoconductivity in monolayer MoS2. Phys Rev Lett 2014;113:166801.
Singh A, Moody G, Tran K, et al. Trion formation dynamics in monolayer transition metal dichalcogenides. Phys Rev B 2016;93:041401.
Krasnok A, Lepeshov S, Alu A. Nanophotonics with 2D transition metal dichalcogenides [Invited]. Opt Express 2018;26:15972–94.
Srivastava A, Sidler M, Allain AV, et al. Optically active quantum dots in monolayer WSe2. Nat Nanotechnol 2015;10:491–6.
He Y-M, Clark G, Schaibley JR, et al. Single quantum emitters in monolayer semiconductors. Nat Nanotechnol 2015;10:497–502.
Chakraborty C, Kinnischtzke L, Goodfellow KM, Beams R, Vamivakas AN. Voltage-controlled quantum light from an atomically thin semiconductor. Nat Nanotechnol 2015;10:507–11.
Mak KF, He K, Shan J, Heinz TF. Control of valley polarization in monolayer MoS2 by optical helicity. Nat Nanotechnol 2012;7:494–8.
Zeng H, Dai J, Yao W, Xiao D, Cui X. Valley polarization in MoS2 monolayers by optical pumping. Nat Nanotechnol 2012;7:490–3.
Cao T, Wang G, Han W, et al. Valley-selective circular dichroism of monolayer molybdenum disulphide. Nat Commun 2012;3:887.
Kim H, Ahn GH, Cho J, et al. Synthetic WSe2 monolayers with high photoluminescence quantum yield. Sci Adv 2019;5:eaau4728.
Edelberg D, Rhodes D, Kerelsky A, et al. Hundredfold enhancement of light emission via defect control in monolayer transition-metal dichalcogenides. arXiv preprint arXiv:1805.00127;2018.
Schneider C, Glazov MM, Korn T, Hofling S, Urbaszek B. Two-dimensional semiconductors in the regime of strong light-matter coupling. Nat Commun 2018;9:2695.
Stier AV, Wilson NP, Clark G, Xu X, Crooker SA. Probing the influence of dielectric environment on excitons in monolayer WSe2: insight from high magnetic fields. Nano Lett 2016;16:7054–60.
Wang G, Chernikov A, Glazov MM, et al. Colloquium: excitons in atomically thin transition metal dichalcogenides. Rev Mod Phys 2018;90:021001.
Chernikov A, Berkelbach TC, Hill HM, et al. Exciton binding energy and nonhydrogenic rydberg series in monolayer WS2. Phys Rev Lett 2014;113:076802.
Hanbicki AT, Currie M, Kioseoglou G, Friedman AL, Jonker BT. Measurement of high exciton binding energy in the monolayer transition-metal dichalcogenides WS2 and WSe2. Solid State Commun 2015;203:16–20.
Miller RC, Kleinman DA, Tsang WT, Gossard AC. Observation of the excited level of excitons in GaAs quantum wells. Phys Rev B 1981;24:1134–6.
Greene RL, Bajaj KK, Phelps DE. Energy levels of Wannier excitons in GaAs – Ga1-xAlxAs quantum-well structures. Phys Rev B 1984;29:1807–12.
Ugeda MM, Bradley AJ, Shi S-F, et al. Giant bandgap renormalization and excitonic effects in a monolayer transition metal dichalcogenide semiconductor. Nat Mater 2014;13:1091.
Wang G, Marie X, Gerber I, et al. Giant enhancement of the optical second-harmonic emission of WSe2 monolayers by laser excitation at exciton resonances. Phys Rev Lett 2015;114:097403.
Qiu DY, da Jornada FH, Louie SG. Optical spectrum of MoS2: many-body effects and diversity of exciton states. Phys Rev Lett 2013;111:216805.
Hao K, Specht JF, Nagler P, et al. Neutral and charged inter-valley biexcitons in monolayer MoSe2. Nat Commun 2017;8:15552.
Ye Z, Waldecker L, Ma EY, et al. Efficient generation of neutral and charged biexcitons in encapsulated WSe2 monolayers. Nat Commun 2018;9:3718.
Mak KF, Shan J. Photonics and optoelectronics of 2D semiconductor transition metal dichalcogenides. Nat Photonics 2016;10:216–26.
Wang QH, Kalantar-Zadeh K, Kis A, Coleman JN, Strano MS. Electronics and optoelectronics of two-dimensional transition metal dichalcogenides. Nat Nanotechnol 2012;7:699–712.
Liu X, Galfsky T, Sun Z, et al. Strong light–matter coupling in two-dimensional atomic crystals. Nat Photonics 2014;9:30–4.
Fogler MM, Butov LV, Novoselov KS. High-temperature superfluidity with indirect excitons in van der Waals heterostructures. Nat Commun 2014;5:4555.
Wang H, Zhang C, Chan W, Manolatou C, Tiwari S, Rana F. Radiative lifetimes of excitons and trions in monolayers of the metal dichalcogenide MoS2. Phys Rev B 2016;93:045407.
Palummo M, Bernardi M, Grossman JC. Exciton radiative lifetimes in two-dimensional transition metal dichalcogenides. Nano Lett 2015;15:2794–800.
Sun D, Rao Y, Reider GA, et al. Observation of rapid exciton–exciton annihilation in monolayer molybdenum disulfide. Nano Lett 2014;14:5625–9.
Kumar N, Cui Q, Ceballos F, He D, Wang Y, Zhao H. Exciton-exciton annihilation in MoSe2 monolayers. Phys Rev B 2014;89:125427.
Mouri S, Miyauchi Y, Toh M, Zhao W, Eda G, Matsuda K. Nonlinear photoluminescence in atomically thin layered WSe2 arising from diffusion-assisted exciton-exciton annihilation. Phys Rev B 2014;90:155449.
Robert C, Lagarde D, Cadiz F, et al. Exciton radiative lifetime in transition metal dichalcogenide monolayers. Phys Rev B 2016;93:205423.
Moody G, Dass CK, Hao K, et al. Intrinsic homogeneous linewidth and broadening mechanisms of excitons in monolayer transition metal dichalcogenides. Nat Commun 2015;6:8315.
Jakubczyk T, Delmonte V, Koperski M, et al. Radiatively limited dephasing and exciton dynamics in MoSe2 monolayers revealed with four-wave mixing microscopy. Nano Lett 2016;16:5333–9.
Jin C, Kim J, Wu K, et al. On optical dipole moment and radiative recombination lifetime of excitons in WSe2. Adv Funct Mater 2017;27:1601741.
Shi H, Yan R, Bertolazzi S, et al. Exciton dynamics in suspended monolayer and few-layer MoS2 2D crystals. ACS Nano 2013;7:1072–80.
Kleemann M-E, Chikkaraddy R, Alexeev EM, et al. Strong-coupling of WSe2 in ultra-compact plasmonic nanocavities at room temperature. Nat Commun 2017;8:1296.
Stührenberg M, Munkhbat B, Baranov DG, et al. Strong light–matter coupling between plasmons in individual gold Bi-pyramids and excitons in mono- and multilayer WSe2. Nano Lett 2018;18:5938–45.
Koperski M, Nogajewski K, Arora A, et al. Single photon emitters in exfoliated WSe2 structures. Nat Nanotechnol 2015;10:503–6.
Tonndorf P, Schmidt R, Schneider R, et al. Single-photon emission from localized excitons in an atomically thin semiconductor. Optica 2015;2:347–52.
Palacios-Berraquero C, Kara DM, Montblanch AR-P, et al. Large-scale quantum-emitter arrays in atomically thin semiconductors. Nat Commun 2017;8:15093.
Lodahl P, Mahmoodian S, Stobbe S. Interfacing single photons and single quantum dots with photonic nanostructures. Rev Mod Phys 2015;87:347.
Iff O, Lundt N, Betzold S, et al. Deterministic coupling of quantum emitters in WSe2 monolayers to plasmonic nanocavities. Opt Express 2018;26:25944–51.
Tripathi LN, Iff O, Betzold S, et al. Spontaneous emission enhancement in strain-induced WSe2 monolayer-based quantum light sources on metallic surfaces. ACS Photonics 2018;5:1919–26.
Xiao D, Liu G-B, Feng W, Xu X, Yao W. Coupled spin and valley physics in monolayers of MoS2 and other group-VI dichalcogenides. Phys Rev Lett 2012;108:196802.
Gunawan O, Shkolnikov YP, Vakili K, Gokmen T, De Poortere EP, Shayegan M. Valley susceptibility of an interacting two-dimensional electron system. Phys Rev Lett 2006;97:186404.
Shkolnikov Y, De Poortere E, Tutuc E, Shayegan M. Valley splitting of AlAs two-dimensional electrons in a perpendicular magnetic field. Phys Rev Lett 2002;89:226805.
Jha PK, Shitrit N, Ren X, Wang Y, Zhang X. Spontaneous exciton valley coherence in transition metal dichalcogenide monolayers interfaced with an anisotropic metasurface. Phys Rev Lett 2018;121:116102.
Sallen G, Bouet L, Marie X, et al. Robust optical emission polarization in MoS2 monolayers through selective valley excitation. Phys Rev B 2012;86:081301.
Bellus MZ, Ceballos F, Chiu H-Y, Zhao H. Tightly bound trions in transition metal dichalcogenide heterostructures. ACS Nano 2015;9:6459–64.
Mouri S, Miyauchi Y, Matsuda K. Tunable photoluminescence of monolayer MoS2 via chemical doping. Nano Lett 2013;13:5944–8.
Rivera P, Schaibley JR, Jones AM, et al. Observation of long-lived interlayer excitons in monolayer MoSe2–WSe2 heterostructures. Nat Commun 2015;6:6242.
Singh A, Tran K, Kolarczik M, et al. Long-lived valley polarization of intravalley trions in monolayer WSe2. Phys Rev Lett 2016;117:257402.
Song X, Xie S, Kang K, Park J, Sih V. Long-lived hole spin/valley polarization probed by Kerr rotation in monolayer WSe2. Nano Lett 2016;16:5010–4.
Plechinger G, Korn T, Lupton JM. Valley-polarized exciton dynamics in exfoliated monolayer WSe2. J Phys Chem C 2017;121:6409–13.
Poellmann C, Steinleitner P, Leierseder U, et al. Resonant internal quantum transitions and femtosecond radiative decay of excitons in monolayer WSe2. Nat Mater 2015;14:889–93.
Arcari M, Söllner I, Javadi A, et al. Near-unity coupling efficiency of a quantum emitter to a photonic crystal waveguide. Phys Rev Lett 2014;113:093603.
Ding X, He Y, Duan Z-C, et al. On-demand single photons with high extraction efficiency and near-unity indistinguishability from a resonantly driven quantum dot in a micropillar. Phys Rev Lett 2016;116:020401.
Somaschi N, Giesz V, De Santis L, et al. Near-optimal single-photon sources in the solid state. Nat Photonics 2016;10:340–5.
Novotny L, Hecht B. Principles of nano-optics. Cambridge, UK, Cambridge University Press, 2012.
Cai T, Kim J-H, Yang Z, Dutta S, Aghaeimeibodi S, Waks E. Radiative enhancement of single quantum emitters in WSe2 monolayers using site-controlled metallic nanopillars. ACS Photonics 2018;5:3466–71.
Luo Y, Shepard GD, Ardelean JV, et al. Deterministic coupling of site-controlled quantum emitters in monolayer WSe2 to plasmonic nanocavities. Nat Nanotechnol 2018;13:1137–42.
Russell KJ, Liu T-L, Cui S, Hu EL. Large spontaneous emission enhancement in plasmonic nanocavities. Nat Photonics 2012;6:459–62.
Hu S, Khater M, Salas-Montiel R, et al. Experimental realization of deep-subwavelength confinement in dielectric optical resonators. Sci Adv 2018;4:eaat2355.
Robinson JT, Manolatou C, Chen L, Lipson M. Ultrasmall mode volumes in dielectric optical microcavities. Phys Rev Lett 2005;95:143901.
Choi H, Heuck M, Englund D. Self-similar nanocavity design with ultrasmall mode volume for single-photon nonlinearities. Phys Rev Lett 2017;118:223605.
Sauvan C, Hugonin J-P, Maksymov I, Lalanne P. Theory of the spontaneous optical emission of nanosize photonic and plasmon resonators. Phys Rev Lett 2013;110:237401.
Kristensen PT, Hughes S. Modes and mode volumes of leaky optical cavities and plasmonic nanoresonators. ACS Photonics 2014;1:2–10.
Alù A, Engheta N. Tuning the scattering response of optical nanoantennas with nanocircuit loads. Nat Photonics 2008;2:307–10.
Monticone F, Argyropoulos C, Alu A. Optical antennas: controlling electromagnetic scattering, radiation, and emission at the nanoscale. IEEE Antennas Propag Mag 2017;59:43–61.
Kuttge M, García de Abajo FJ, Polman A. Ultrasmall mode volume plasmonic nanodisk resonators. Nano Lett 2009;10:1537–41.
Akselrod GM, Argyropoulos C, Hoang TB, et al. Probing the mechanisms of large Purcell enhancement in plasmonic nanoantennas. Nat Photonics 2014;8:835–40.
Wang C, Badolato A, Wilson-Raea I, Petroff PM, Hu E. Optical properties of single InAs quantum dots in close proximity to surfaces. Appl Phys Lett 2004;85:3423–5.
Zhang H, Huo Y, Lindfors K, et al. Narrow-line self-assembled GaAs quantum dots for plasmonics. Appl Phys Lett 2015;106:101110.
Farahani JN, Pohl DW, Eisler H-J, Hecht B. Single quantum dot coupled to a scanning optical antenna: a tunable superemitter. Phys Rev Lett 2005;95:017402.
Lyamkina A, Schraml K, Regler A, et al. Monolithically integrated single quantum dots coupled to bowtie nanoantennas. Opt Express 2016;24:28936–44.
Pfeiffer M, Lindfors K, Zhang H, et al. Eleven nanometer alignment precision of a plasmonic nanoantenna with a self-assembled GaAs quantum dot. Nano Lett 2013;14:197–201.
Regler A, Schraml K, Lyamkina A, et al. Emission redistribution from a quantum dot-bowtie nanoantenna. J Nanophotonics 2016;10:033509.
Lee B, Park J, Han GH, et al. Fano resonance and spectrally modified photoluminescence enhancement in monolayer MoS2 integrated with plasmonic nanoantenna array. Nano Lett 2015;15:3646–53.
Butun S, Tongay S, Aydin K. Enhanced light emission from large-area monolayer MoS2 using plasmonic nanodisc arrays. Nano Lett 2015;15:2700–4.
Johnson AD, Cheng F, Tsai Y, Shih CK. Giant enhancement of defect-bound exciton luminescence and suppression of band-edge luminescence in monolayer WSe2-Ag plasmonic hybrid structures. Nano Lett 2017;17:4317–22.
Eggleston MS, Desai SB, Messer K, et al. Ultrafast spontaneous emission from a slot-antenna coupled WSe2 monolayer. ACS Photonics 2018;5:2701–5.
Dutta S, Cai T, Buyukkaya MA, Barik S, Aghaeimeibodi S, Waks E. Coupling quantum emitters in WSe2 monolayers to a metal-insulator-metal waveguide. Appl Phys Lett 2018;113:191105.
Palacios E, Park S, Butun S, Lauhon L, Aydin K. Enhanced radiative emission from monolayer MoS2 films using a single plasmonic dimer nanoantenna. Appl Phys Lett 2017;111:031101.
Cai T, Dutta S, Aghaeimeibodi S, et al. Coupling emission from single localized defects in two-dimensional semiconductor to surface plasmon polaritons. Nano Lett 2017;17:6564–8.
Amani M, Lien D-H, Daisuke Kiriya D, et al. Near-unity photoluminescence quantum yield in MoS2. Science 2015;350:1065–8.
Li Z, Liu C, Rong X, et al. Tailoring MoS2 valley-polarized photoluminescence with super chiral near-field. Adv Mater 2018;30:1801908.
Chervy T, Azzini S, Lorchat E, et al. Room temperature chiral coupling of valley excitons with spin-momentum locked surface plasmons. ACS Photonics 2018;5:1281–7.
Chen H, Liu M, Xu L, Neshev DN. Valley-selective directional emission from a transition-metal dichalcogenide monolayer mediated by a plasmonic nanoantenna. Beilstein J Nanotechnol 2018;9:780–8.
Reithmaier JP, Sęk G, Löffler A, et al. Strong coupling in a single quantum dot–semiconductor microcavity system. Nature 2004;432:197–200.
Dintinger J, Klein S, Bustos F, Barnes WL, Ebbesen T. Strong coupling between surface plasmon-polaritons and organic molecules in subwavelength hole arrays. Phys Rev B 2005;71:035424.
Ezawa M. Valley-polarized metals and quantum anomalous Hall effect in silicene. Phys Rev Lett 2012;109:055502.
Tahir M, Manchon A, Sabeeh K, Schwingenschlögl U. Quantum spin/valley Hall effect and topological insulator phase transitions in silicene. Appl Phys Lett 2013;102:162412.
Lee J, Mak KF, Shan J. Electrical control of the valley Hall effect in bilayer MoS2 transistors. Nat Nanotechnol 2016;11:421–5.
Guinea F, Katsnelson M, Geim A. Energy gaps and a zero-field quantum Hall effect in graphene by strain engineering. Nat Phys 2010;6:30–3.
Zhang Y, Tan Y-W, Stormer HL, Kim P. Experimental observation of the quantum Hall effect and Berry’s phase in graphene. Nature 2005;438:201–4.
Petersen J, Volz J, Rauschenbeutel A. Chiral nanophotonic waveguide interface based on spin-orbit interaction of light. Science 2014;346:67–71.
Mueller JPB, Capasso F. Asymmetric surface plasmon polariton emission by a dipole emitter near a metal surface. Phys Rev B 2013;88:121410.
Rodríguez-Fortuño FJ, Marino G, Ginzburg P, et al. Near-field interference for the unidirectional excitation of electromagnetic guided modes. Science 2013;340:328–30.
Coles RJ, Price DM, Dixon JE, et al. Chirality of nanophotonic waveguide with embedded quantum emitter for unidirectional spin transfer. Nat Commun 2016;7:11183.
Sollner I, Mahmoodian S, Hansen SL, et al. Deterministic photon-emitter coupling in chiral photonic circuits. Nat Nanotechnol 2015;10:775–8.
Wei H, Ratchford D, Li X, Xu H, Shih C-K. Propagating surface plasmon induced photon emission from quantum dots. Nano Lett 2009;9:4168–71.
Akimov AV, Mukherjee A, Yu CL, et al. Generation of single optical plasmons in metallic nanowires coupled to quantum dots. Nature 2007;450:402–6.
Gong S-H, Alpeggiani F, Sciacca B, Garnett EC, Kuipers L. Nanoscale chiral valley-photon interface through optical spin-orbit coupling. Science 2018;359:443–7.
Schuller JA, Karaveli S, Schiros T, et al. Orientation of luminescent excitons in layered nanomaterials. Nat Nanotechnol 2013;8:271–6.
Sun L, Wang C-Y, Krasnok A, et al. Separation of valley excitons in a MoS2 monolayer using a subwavelength asymmetric groove array. Nat Photonics 2019;13:180–4.
Hong X, Kim J, Shi S-F, et al. Ultrafast charge transfer in atomically thin MoS2/WS2 heterostructures. Nat Nanotechnol 2014;9:682–6.
Kozawa D, Carvalho A, Verzhbitskiy I, et al. Evidence for fast interlayer energy transfer in MoSe2/WS2 heterostructures. Nano Lett 2016;16:4087–93.
Chen H, Wen X, Zhang J, et al. Ultrafast formation of interlayer hot excitons in atomically thin MoS2/WS2 heterostructures. Nat Commun 2016;7:12512.
He J, Kumar N, Bellus KZ, et al. Electron transfer and coupling in graphene–tungsten disulfide van der Waals heterostructures. Nat Commun 2014;5:5622.
Ceballos F, Bellus MZ, Chiu H-Y, Zhao H. Ultrafast charge separation and indirect exciton formation in a MoS2–MoSe2 van der Waals heterostructure. ACS Nano 2014;8:12717–24.
Chiu M-H, Zhang C, Shiu H-W, et al. Determination of band alignment in the single-layer MoS2/WSe2 heterojunction. Nat Commun 2015;6:7666.
Claassen M, Jia C, Moritz B, Devereaux TP. All-optical materials design of chiral edge modes in transition-metal dichalcogenides. Nat Commun 2016;7:13074.
Iadecola T, Campbell D, Chamon C, et al. Materials design from nonequilibrium steady states: driven graphene as a tunable semiconductor with topological properties. Phys Rev Lett 2013;110:176603.
Perez-Piskunow PM, Usaj G, Balseiro CA, Foa Torres LEF. Floquet chiral edge states in graphene. Phys Rev B 2014;89:121401.
Yu H, Liu G-B, Tang J, Xu X, Yao W. Moiré excitons: from programmable quantum emitter arrays to spin-orbit–coupled artificial lattices. Sci Adv 2017;3:e1701696.
Wu F, Lovorn T, MacDonald AH. Theory of optical absorption by interlayer excitons in transition metal dichalcogenide heterobilayers. Phys Rev B 2018;97:035306.
Note that in literature there are slightly different definitions of the Purcell factor. Here we follow the notation somehow prevalent in the TMDs community ,  and define